- Email: [email protected]

Contents lists available at ScienceDirect

Optics Communications journal homepage: www.elsevier.com/locate/optcom

Nonlinear optical absorption in parabolic quantum well via two-photon absorption process Huynh Vinh Phuc a,c,n, Nguyen Ngoc Hieu a, Le Dinh b, Tran Cong Phong b a

Institute of Research and Development, Duy Tan University, Da Nang, Viet Nam Center for Theoretical and Computational Physics, Hue University, Hue, Viet Nam c Department of Physics, Dong Thap University, Dong Thap, Viet Nam b

art ic l e i nf o

a b s t r a c t

Article history: Received 8 August 2014 Received in revised form 29 August 2014 Accepted 1 September 2014 Available online 16 September 2014

We theoretically study the nonlinear optical absorption phenomenon in a GaAs/GaAlAs parabolic quantum well via investigating the phonon-assisted cyclotron resonance (PACR) effect. We ﬁnd that the two-photon absorption process (nonlinear) is comparable with the one-photon process (linear), and cannot be neglected in studying PACR effect. The additional peaks in the absorption spectrum due to transitions between Landau levels and electric subband energy accompanied by emission and absorption of LO-phonon are indicated. PACR behavior is strongly affected by the magnetic ﬁeld, the temperature and the conﬁnement frequency. The present work obtains an usefully resonant condition which is more general than and includes the previous resonant behaviors. & 2014 Elsevier B.V. All rights reserved.

Keywords: Nonlinear optics Phonon-assisted cyclotron resonance Linewidth

1. Introduction The multi-photon absorption process, or a nonlinear phenomenon, has been studied in a large number of papers in recent years [1–7]. In these papers, the ﬁrst- and second-orders of the nonlinear optical conductivity have been obtained using the projectiondiagram method. Although these results are very clear in physical interpretation and useful in the study of optical conductivity in lowdimensional systems, their analytical calculations are quite complicated. Therefore, these results have not been applied to investigate the nonlinear phenomenon, especially, in numerical calculations. In the other works, using different methods, many researchers have succeeded in studying the linear and nonlinear optical absorptions in low-dimensional semiconductor quantum systems [8–20]. The results show that the optical absorption coefﬁcients are strongly affected by conﬁnement potential [11,14], structural parameters of the system [8–10,13–18], hydrostatic pressure [16,17,19], and external ﬁelds [12,20]. However, these works only investigated the optical absorption process via one-photon absorption process, the twophoton absorption process is still open for further investigation. Phonon-assisted cyclotron resonance (PACR) has been known as one of the useful tools for investigating transport behaviour of electrons in semiconductor materials under an applied magnetic ﬁeld. This effect indicates the transition of electrons between

Landau levels due to the absorption of photons accompanied with the absorption or emission of phonons. Since the early theoretical predictions [21] and experimental observations [22], the cyclotron resonance and PACR have been studied both theoretically and experimentally in bulk semiconductors [23–26], in quantum wells [27–32], in quantum wires [33–35], and in quantum dots [36]. However, the study of nonlinear PACR in PQW has not been found. It is known that in GaAs/GaAlAs systems, electron interaction with polar phonon modes is of great importance [29]. Therefore, the purpose of the present work is to investigate the effects of the magnetic ﬁeld, the temperature and the conﬁnement frequency on the linear and nonlinear optical absorption spectrum in GaAs/ Ga1 xAlxAs PQW in the presence of electron–LO phonon interaction. Besides, the present work also obtains an useful resonant behaviour which expresses the phonon-assisted cyclotron resonance condition, including the other types of resonances, such as the optically detected electrophonon resonance [37,38] and the optically detected magnetophonon resonance [39]. The paper is organized as follows: in Section 2, the theoretical framework used in calculations and the analytical results are presented. The discussion of the results is given in Section 3. Finally, the conclusion is given in Section 4.

2. Theoretical framework and analytical results n

Corresponding author at: Department of Physics, Dong Thap University, Dong Thap, Viet Nam. Tel.: þ 84 67 3882919. E-mail address: [email protected] (H.V. Phuc). http://dx.doi.org/10.1016/j.optcom.2014.09.004 0030-4018/& 2014 Elsevier B.V. All rights reserved.

When an electromagnetic wave characterized by a timedependence electric ﬁeld of amplitude F0 and angular frequency

38

H.V. Phuc et al. / Optics Communications 335 (2015) 37–41

Ω is applied to a semiconductor system, the optical absorption power is given by [31] pﬃﬃﬃ F2 ε ð1Þ PðΩÞ ¼ 0 ∑W i f i ; 8π i where ε is the dielectric constant of the medium, fi is the electron distribution function, and Wi is the transition probability. The sum is taken over all the initial states i of electrons. The transition probability of absorbing photon with simultaneously absorbing and/or emitting phonon W i8 can be written as [31,40] þ1 2π 1 a0 q ? 2ℓ W i8 ¼ ∑∑jM fi j2 ∑ 2 ℏ f q 2 ℓ ¼ 1 ðℓ!Þ δðEf Ei 8 ℏωq ℓℏΩÞ;

ð2Þ

where the upper ð Þ and lower sign ð þ Þ refer to the phonon absorption and phonon emission, respectively, Mﬁ is the transition matrix element of the electron–phonon interaction, a0 is the laser dressing parameter, Ei EN;n and Ef EN0 ;n0 are the energy initial and ﬁnal states of the electron, respectively, and q ¼ ðqz ; q ? Þ is the phonon wave vector. We consider a PQW, in which electron system is conﬁned in z-direction by the potential UðzÞ ¼ mn ω2z z2 =2, where ωz is the conﬁnement frequency. When a static magnetic ﬁeld B ¼ ð0; 0; BÞ is applied to system, the normalized eigenfunctions in the Landau gauge for the vector potential A ¼ ð0; Bx; 0Þ and the corresponding energy are given by [41] 1 jN; n; ky 〉 ¼ pﬃﬃﬃﬃﬃ expðiky yÞϕN ðx x0 Þψ n ðzÞ; Ly 1 EN;n ¼ N þ ℏωc þ εn ; 2

ð3Þ

jJ NN0 ðq ? Þj2 ¼

ð4Þ

1 εn ¼ n þ ℏωz ; 2

n ¼ 0; 1; 2; …;

ð6Þ

where Hn(x) is the nth Hermite polynomial and az ¼ ðℏ=mn ωz Þ1=2 . The matrix elements for electron-conﬁned LO-phonon interaction in PQW in the presence of magnetic ﬁeld can be written as 2 M fi ¼ jV m ðqÞj2 jJ 0 ðq Þj2 jJ 0 ðq Þj2 nn z NN ? ðN Li þ 1=2 8 1=2Þδkz 0 ;kz 7 qz ; ð7Þ where NLi is the distribution function of conﬁned LO-phonon for frequency ωq ¼ ωLi , and the coupling function is given by [42] !1 e2 ℏωLi 1 1 m2 π 2 2 2 jV m ðqÞj ¼ q? þ 2 ; m ¼ 1; 2; 3; …; ε0 di χ 1i χ 0i d i

ð8Þ with ε0 is the permittivity of free space, χ 1i (χ0i) and di are the high (low) frequency dielectric constants and the thickness of region i of quantum well, respectively, and jJ nn0 ðqzm Þj2 ¼

0 n! a2z q2zm =2 2 2 e ðaz qzm =2Þn n n0 !

ð9Þ

0 N! a2c q2 =2 2 2 ? e ðac q ? =2ÞN N N0 ! h i2 N 2 2 LN0 ðac q ? =2Þ ; N r N 0 ; N

ð10Þ

N;N 0 ;n;n0

þ ðNLi þ1Þδðpℏωc þ Δεn0 n þ ℏωLi ℏΩÞ þ ðN þ N 0 þ 1Þ

a20 ½NLi δðpℏωc þ Δεn0 n 8a2c

ℏωLi 2ℏΩÞ þ ðN Li þ 1Þδðpℏωc þ Δεn0 n þ ℏωLi 2ℏΩÞg;

ð11Þ

here we denoted p ¼ N0 N (is an integer), and Δεn0 n ¼ εn0 εn ¼ ðn0 nÞℏωz . In Eq. (11), the overlap integral I nn0 is deﬁned as 2 J 0 mπ ; nn d i m ¼ 1;2;3;… ∑

ð12Þ

and

n

where m is the effective mass of a conduction electron, N and n are the Landau level index and the level quantized number in z-direction, respectively; and ωc ¼ eB=mn is the cyclotron frequency. Also, ϕN ðx x0 Þ represents the harmonic oscillator wave function, centered at x0 ¼ ky =mn ωc . Here ky and Ly are the wave vector and the normalization length in y-direction, respectively. The radius of the orbit in the ðx; yÞ plane is ac ¼ ðℏ=mn ωc Þ1=2 . In Eqs. (3) and (4), the one-electron normalized eigenfunctions and the corresponding eigenvalues in the conduction band are, respectively, given by 1=2 1 z2 z ψ n ðzÞ ¼ exp 2 H n ; ð5Þ n pﬃﬃﬃ az 2az 2 n! π az

n r n0 ;

where we have denoted qzm ¼ mπ=di , and LM N ðxÞ is the associated Laguerre polynomials. The transition probability in Eq. (2) contains contributions of absorption process of ℓ-photons. In this paper, we restrict ourselves to considering the process of absorbing two photons ðℓ ¼ 1; 2Þ. Using Eq. (1) and making a straight forward calculation of probability with the use of matrix element for conﬁned LOphonon scattering (Eq. (7)), we obtain the expression for the optical absorption power in PQW in the case of non-degenerate electron gas

PðΩÞ ¼ AðΩ; ωc Þ ∑ jI nn0 je EN;n =kB T ½N Li δðpℏωc þ Δεn0 n ℏωLi ℏΩÞ

I nn0 ¼

N ¼ 0; 1; 2; …;

n 2 2 2 Ln0 ðaz qzm =2Þ ; n

AðΩ; ωc Þ ¼

pﬃﬃﬃ F 20 εne V 20 a20 e2 ωLi 1 1 ; 3 6 128π Lz di λac ε0 χ 1i χ 0i

λ ¼ ∑ e EN;n =kB T N;n

with ne is the electron concentration, kB is the Boltzmann constant, T is the temperature. In Eq. (11), the delta functions present the energy conservation law. This implies that when an electron undergoes a collision by absorbing photon energy, its energy can only change by an amount equal to the energy of a phonon involved in the transitions. The energy-conservation delta functions in Eq. (11) show resonant behaviour at the PARC condition for PQW based on the following selection rule of transition condition: ℓℏΩ ¼ pℏωc þ Δεn0 n 7 ℏωLi :

ð13Þ

This condition predicates that the PACR is affected by both Landau and electric subband levels. In the case of transitions without electric subband levels, this equation reduces to ℓℏΩ ¼ pℏωc 7 ℏωLi . This is the pure PACR condition which is only affected by the Landau levels [31]. Furthermore, we also see that the transition condition in Eq. (13) can include the other resonant behaviours, such as the optically detected electrophonon resonance (ODEPR) [37,38], and the optically detected magnetophonon resonance (ODMPR) [39]. Indeed, being only affected by the electric subband levels, ODEPR, which satisﬁes the condition ℏΩ ¼ Δεn0 n 7 ℏωLi , is the speciﬁc case of PACR condition in the case of ℓ ¼ 1; p ¼ 0. Similarly, satisfying the condition pℏωc ¼ ℏωLi þ Δεn0 n 7 ℏΩ, ODMPR is the speciﬁc case of PACR condition with ℓ ¼ 1. Therefore, it can be seen that our PACR condition is more general than the previous ones. Following the collision broadening model, the delta functions in Eq. (11) are replaced with Lorentzians [43] δðZ ℓ7 Þ ¼

ℏΓ ℓ8 1 ; 7 2 π ðZ ℓ Þ þ ℏ2 ðΓ ℓ8 Þ2

ð14Þ

H.V. Phuc et al. / Optics Communications 335 (2015) 37–41

where Z ℓ7

¼ pℏωc þ Δεn0 n 7 ℏωLi ℓℏΩ

ðℓ ¼ 1; 2Þ;

ð15Þ

and Γ ℓ8 is the inverse relaxation time of electrons jI nn0 je2 ωLi 1 1 ðN Li þ 1=2 8 1=2Þ; p a 0: ðΓ ℓ8 Þ2 ¼ 2 8π di ℏpε0 χ 1i χ 0i

ð16Þ

The present result yields a more speciﬁc and signiﬁcant interpretation of the electronic processes for emission and absorption of phonons and photons under the applied magnetic ﬁeld in GaAs/Ga1 xAlxAs PQW. In the next section, we will consider the numerical evaluation in more detail.

3. Numerical results and discussion

Therefore, the nonlinear absorption process is strong enough to be detected in PACR. In the barrier Ga0.6Al0.4As, the phenomenon occurs similarly, but the resonance peaks seem to give a red-shift. This resulted in the effective mass of electron and conﬁned LO-phonon energy which are modiﬁed in Ga0.6Al0.4As. In detail, for x ¼0.4, the effective mass mn ¼ 0:1me leading to cyclotron energy ℏωc ¼ 10:46 meV, and ℏωLi ¼ 39:39 meV. Therefore, the resonant peak occurring at ℏΩ ¼ 64:4 meV satisﬁes the condition Ω ¼ pωc þωz þ ωLi , with p ¼1. This value of the resonant peak is smaller than that in GaAs (66.40 meV). This explains the red-shift behavior of the absorption spectrum in the barrier Ga0.6Al0.4As. The others peaks of the dashed line can be explained similarly. In Fig. 2, we depict the absorption power in the well GaAs as functions of photon energy for different values of magnetic ﬁeld. It is possible to see that the increase in the value of magnetic ﬁeld leads to a blue-shift of the resonant peaks. The physical meaning of this phenomenon is that when the magnetic ﬁeld increases, the Landau level separation becomes larger resulting in the increase of the value of absorbed photon energy. Fig. 3 shows the dependence of PACR absorption spectrum on the temperature. We can see from the ﬁgure that the PACR peaks are located at the same position but the peak values of absorption power are seen to increase with the temperature. As the temperature increases, the electron–phonon scattering increases, leading to a general increase in the temperature of absorption power. Fig. 4 shows the dependence of PACR absorption spectrum on the conﬁnement frequency. In the ﬁgure, when the conﬁnement frequency increases, the PACR peaks are seen to shift to the large region of the photon energy (blue-shift). As the conﬁnement frequency increases, the electric subband separation energy increases, leading to the increasing of the value of absorbed photon energy. For the PACR-linewidth, using proﬁle method [45] we obtain the magnetic ﬁeld dependence of the PACR-linewidth, as shown in Fig. 5. It can be found that both the well and barrier PACRlinewidth increase with increasing magnetic ﬁeld B. The reason for this is that the electron–phonon interaction increases when magnetic ﬁeld increases. This result is in good agreement with the results of previous papers [25–27,32,34]. The physical meaning of this phenomenon can be explained as follows: when magnetic ﬁeld B increases, the cyclotron radius ac reduces, the conﬁnement of electron increases, the probability of electron–phonon scattering increases, leading to the increasing of the linewidth. In addition, we can also see from the ﬁgure that PACR-linewidth varies with the square root of magnetic ﬁeld, agreeing with the previous result [27]. Besides, the linewidth in nonlinear absorption process is about 51% of that in linear one for the well and 49% for

P arb. units

P arb. units

For the numerical calculations, we take the following values as the input parameter [13,37,44]: ε ¼ 12:5, χ 1 ¼ 10:89, χ 0 ¼ 13:18, mn ¼ 0:067me , me being the mass of free electron, ℏω0 ¼ 36:25 meV, ne ¼ 1023 m 3 , and a0 ¼ 5 nm for GaAs, and mn ¼ ð0:067 þ0:083xÞme , ℏωLi ¼ ð36:25 þ 1:83x þ 17:12x2 5:11x3 Þ meV, χ 0i ¼ 13:18 3:12x, χ 1i ¼ 10:89 2:73x for Ga1 xAlxAs [42]. In Fig. 1 we show the dependence of the absorption power on photon energy at B ¼9 T, which leads to the cyclotron energy ℏωc ¼ 15:65 meV in the well GaAs and 10.46 meV in the barrier Ga0.6Al0.4As, respectively. These peaks are due to PACR, which represents resonance transfer of electrons with absorption of photons accompanied with the absorption/emission of phonons. Depending upon the Landau level and electric subband separations, photon, and phonon energies, the PACR transitions have various types [29]. For a magnetic ﬁeld B¼ 9 T, the cyclotron energy is smaller than the LO-phonon energy, the transitions correspond to the type 2 in Ref. [29]. Using the computational method, we easily determine that the peaks at ℏΩ ¼ 66:40 meV, 82.05 meV and 97.70 meV of the solid line satisfy the condition Ω ¼ pωc þ ωz þ ω0 , with p ¼1, 2 and 3, respectively. These three peaks correspond to the one-photon process (linear phenomenon). Moreover, the peak value of absorption power at p ¼2 and 3 is about 52% and 34%, respectively, of that at p ¼1. At ℏΩ ¼ 33:20 meV, 41.03 meV, and 48.85 meV, the peaks satisfy the condition 2Ω ¼ pωc þ ωz þ ω0 , with p ¼1, 2 and 3, respectively, describing the two-photon process (nonlinear phenomenon). In the nonlinear case, the peak values at p ¼2 and p¼ 3 are about 79% and 73.7%, of that at p ¼1, respectively. Besides, the peak values in the nonlinear process are about 26%, 40%, and 56%, respectively, of that in the linear process at p ¼1,2, and p ¼3.

39

20

40

60

80

100

120

Photon Energy meV Fig. 1. Absorption power as a function of the photon energy in a PQW with a conﬁnement frequency ωz =ω0 ¼ 0:4 at B¼ 9 T, di ¼50 Å, and T ¼77 K. The solid and dashed lines present the absorption power in the well GaAs, and the barrier Ga0.6Al0.4As (x ¼0.4), respectively.

20

40

60 80 Photon Energy meV

100

120

Fig. 2. Absorption power is shown as a function of photon energy for different values of magnetic ﬁeld. The solid, dashed, and dotted curves correspond to B¼ 9 T, 10 T, and 11 T. Here T ¼ 77 K, di ¼50 Å, and ωz =ω0 ¼ 0:4.

40

H.V. Phuc et al. / Optics Communications 335 (2015) 37–41

P arb. units

PACR Linewidth meV

8

- GaAs - Ga0.6 Al0.4 As

7 6 5 4 3 2 1

20

40

60 80 Photon Energy meV

100

50

120

PACR Linewidth meV

P arb. units

60

80

100

120

PACR Linewidth meV

- GaAs - Ga 0.6 Al0.4 As

6

4

2 10

15

20

300

350

400

5 4 3 2 0.2

0.4

0.6

0.8

1.0 z

Fig. 4. Absorption power is shown as a function of photon energy for different values of conﬁnement frequency. The solid, dashed, and dotted curves correspond to ωz =ω0 ¼ 0:4, 0.5, and 0.6. Here B¼ 9 T, di ¼ 50 Å, and T ¼ 77 K.

5

250

- GaAs - Ga0.6 Al0.4 As

Photon Energy meV

8

200

Fig. 6. Dependence of the PACR-linewidth on the temperature at B¼9 T, di ¼50 Å, and ωz =ω0 ¼ 0:4. The circle and rectangular lines present the linewidth in the well GaAs and the barrier Ga0.6Al0.4As, the ﬁlled and empty lines correspond to the linear and nonlinear absorption process, respectively.

6

40

150

Temperature K

Fig. 3. Absorption power is shown as a function of photon energy for different values of temperature. The solid, dashed, and dotted curves correspond to T ¼ 77 K, 150 K, and 300 K. Here B ¼9 T, di ¼ 50 Å, and ωz =ω0 ¼ 0:4.

20

100

25

30

Magnetic field T Fig. 5. Dependence of the PACR-linewidth on the magnetic ﬁeld at T ¼ 77 K, di ¼ 50 Å, and ωz =ω0 ¼ 0:4. The diamond and triangle lines present the linewidth in the well GaAs and the barrier Ga0.6Al0.4As, the ﬁlled and empty lines correspond to the linear and nonlinear absorption process, respectively.

the barrier. Therefore, this result once again shows that the nonlinear absorption process is strong enough to be detected, and cannot be neglected in studying the PACR-linewidth in PQW. Fig. 6 shows the temperature dependence of the PACR-linewidth. It is seen from the ﬁgure that the PACR-linewidth varies with the square root of temperature. This result is in good agreement with the result of the paper of Chaubey and Van Vliet [27]. As the temperature increases, probability of electron–phonon scattering increases, leading to a general increase in the temperature of PACR-linewidth. The

1.2

1.4

1.6

0

Fig. 7. Dependence of the PACR-linewidth on the conﬁnement frequency at B¼ 9 T, di ¼ 50 Å, and T ¼77 K. The square and down-triangle lines present the linewidth in the well GaAs and the barrier Ga0.6Al0.4As, the ﬁlled and empty lines correspond to the linear and nonlinear absorption process, respectively.

linewidth in nonlinear absorption process is about 50% of that in linear one in both the well GaAs and the barrier Ga0.6Al0.4As. Fig. 7 shows the dependence of PACR-linewidth on the conﬁnement frequency at B ¼9 T, and T ¼77 K. From the ﬁgure, we can see that the PACR-linewidth increases with the conﬁnement frequency for both linear and nonlinear absorption process. Furthermore, the PACR-linewith in the linear process varies faster and has a larger value than it does in comparison with the nonlinear process. In this case, the linewidth in the nonlinear absorption process is from about 84% (95%) at ωz =ω0 ¼ 0:2 to 63% (58%) at ωz =ω0 ¼ 1:6 of that in the linear one for the well GaAs (the barrier Ga0.6Al0.4As). Finally, we can see that the PACR-linewidth in the barrier is always smaller than that in the well in each case associated.

4. Conclusion In the present work, we have studied the PACR in GaAs/GaAlAs PQW by considering the two-photon absorption process when electrons interact with LO-phonons. The absorption spectrum satisﬁes the condition ℓℏΩ ¼ pℏωc þΔεn0 n 7 ℏωLi , and can include the other resonant behaviours. The results show that the PACR behaviour is affected by the magnetic ﬁeld, the temperature and conﬁnement frequency. Using proﬁle method, we obtained the PACR-linewidth as proﬁle of the curves. The values of the PACR-linewidth are found

H.V. Phuc et al. / Optics Communications 335 (2015) 37–41

to increase with the increase of magnetic ﬁeld, temperature and conﬁnement frequency. Although being smaller than the linear absorption process, the nonlinear process is strong enough to be detected in PACR, and cannot be neglected in studying the PACRlinewidth. Unfortunately, up to now, there are no relevant experimental result for comparing to our theory. We hope that new experiments will test the validity of our prediction in a very near future. Acknowledgments The authors would like to thank the anonymous reviewers for their helpful and constructive comments that greatly contributed to improving the paper. Appendix A. Supplementary data Supplementary data associated with this paper can be found in the online version at http://dx.doi.org/10.1016/j.optcom.2014.09.004. References [1] [2] [3] [4] [5] [6] [7] [8] [9] [10] [11] [12]

H.J. Lee, N.L. Kang, J.Y. Sug, S.D. Choi, Phys. Rev. B 65 (2002) 195113. N.L. Kang, S.D. Choi, J. Phys. A: Math. Theor. 43 (2010) 165203. N.L. Kang, Y.J. Lee, S.D. Choi, J. Korean Phys. Soc. 58 (2011) 538. N.L. Kang, S.D. Choi, J. Mod. Phys. 2 (2011) 1410. N.L. Kang, S.D. Choi, Prog. Theor. Phys. 125 (2011) 1011. N.L. Kang, S.D. Choi, AIP Adv. 2 (2012) 012161. N.L. Kang, S.-S. Lee, S.D. Choi, AIP Adv. 3 (2013) 072104. A. Keshavarz, M. Karimi, Phys. Lett. A 374 (2010) 2675. L.T.T. Phuong, H.V. Phuc, T.C. Phong, Comput. Mater. Sci. 49 (2010) S260. R. Khordad, S. Tafaroji, Physica E 46 (2012) 84. W. Xie, Opt. Commun. 284 (2011) 5730. F. Ungan, U. Yesilgul, E. Kasapoglu, H. Sari, I. Sokmen, J. Lumin. 132 (2012) 1627.

[13] [14] [15] [16] [17] [18] [19] [20] [21] [22] [23] [24] [25] [26] [27] [28] [29] [30] [31] [32] [33] [34] [35] [36] [37] [38] [39] [40] [41] [42] [43] [44] [45]

41

U. Yesilgul, J. Lumin. 132 (3) (2012) 765. Y. Yakar, B. akr, A. zmen, Opt. Commun. 283 (2010) 1795. E. Ozturk, Y. Ozdemir, Opt. Commun. 294 (2013) 361. R. Restrepo, M. Barseghyan, M. Mora-Ramos, C. Duque, Physica E 51 (2013) 48. H. Baghramyan, M. Barseghyan, A. Kirakosyan, R. Restrepo, C. Duque, J. Lumin. 134 (2013) 594. H. Baghramyan, M. Barseghyan, A. Kirakosyan, R. Restrepo, M. Mora-Ramos, C. Duque, J. Lumin. 145 (2014) 676. V. Mughnetsyan, A. Manaselyan, M. Barseghyan, A. Kirakosyan, J. Lumin. 134 (2013) 24. E.C. Niculescu, N. Eseanu, A. Radu, Opt. Commun. 294 (2013) 276. F.G. Bass, I.B. Levinson, Sov. Phys. JETP 22 (1966) 635. R.C. Enck, A.S. Saleh, H.Y. Fan, Phys. Rev. 182 (1969) 790. Y.J. Cho, S.D. Choi, Phys. Rev. B 49 (1994) 14301. T.M. Rynne, H.N. Spector, J. Appl. Phys. 52 (1981) 393. J.Y. Sug, S.G. Jo, J. Kim, J.H. Lee, S.D. Choi, Phys. Rev. B 64 (2001) 235210. H. Kobori, T. Ohyama, E. Otsuka, J. Phys. Soc. Jpn. 59 (1990) 2141. M.P. Chaubey, C.M. Van Vliet, Phys. Rev. B 34 (1986) 3932. J.S. Bhat, S.S. Kubakaddi, B.G. Mulimani, J. Appl. Phys. 70 (1991) 2216. J.S. Bhat, B.G. Mulimani, S.S. Kubakaddi, Phys. Rev. B 49 (1994) 16459. Y.B. Vasilyev, S.D. Suchalkin, S.V. Ivanov, B.Y. Meltser, P.S. Kop'ev, Phys. Status Solidi B 240 (2003) R8. H.V. Phuc, L. Dinh, T.C. Phong, Superlattices Microstruct. 59 (2013) 77. H.V. Phuc, L.V. Tung, Superlattices Microstruct. 71 (2014) 124. V.A. Margulis, A.V. Shorokhov, Phys. Status Solidi C 1 (2004) 2642. H.V. Phuc, L.T.M. Hue, L. Dinh, T.C. Phong, Superlattices Microstruct. 60 (2013) 508. R. Betancourt-Riera, R. Betancourt-Riera, J.N. Jalil, R. Riera, Physica B 410 (2013) 126. S.-H. Chen, Physica E 43 (2011) 1007. S.C. Lee, J.W. Kang, H.S. Ahn, M. Yang, N.L. Kang, S.W. Kim, Physica E 28 (2005) 402. L.T.T. Phuong, H.V. Phuc, T.C. Phong, Physica E 56 (2014) 102. S.C. Lee, J. Korean Phys. Soc. 51 (2007) 1979. W. Xu, R.A. Lewis, P.M. Koenraad, C.J.G.M. Langerak, J. Phys.: Condens. Matter 16 (2004) 89. R. Haupt, L. Wendler, Solid State Commun. 89 (1994) 741. J. Gong, X.X. Liang, S.L. Ban, J. Appl. Phys. 100 (2006) 023707. M.P. Chaubey, C.M. Van Vliet, Phys. Rev. B 33 (1986) 5617. X. Yu, Y. Yu, Superlattices Microstruct. 62 (2013) 225. T.C. Phong, H.V. Phuc, Mod. Phys. Lett. B 25 (2011) 1003.

Copyright © 2023 C.COEK.INFO. All rights reserved.